E 8M – 04discontinuous yielding to uniform strain hardening. If the must be flat and parallel. For best results, the wedges should betransition occurs over a range of strain, the YPE end point is supported over their entire lengths by the heads of the testingthe intersection between (a) a horizontal line drawn tangent to machine. This requires that liners of several thicknesses bethe curve at the last zero slope and ( b) a line drawn tangent to available to cover the range of specimen thickness. For properthe strain hardening portion of the stress-strain curve at the gripping, it is desirable that the entire length of the serratedpoint of inflection. If there is no point at or near the onset of face of each wedge be in contact with the specimen. Properyielding at which the slope reaches zero, the material has 0 % alignment of wedge grips and liners is illustrated in Fig. 2. ForYPE. short specimens and for specimens of many materials, it is 3.1.5 uniform elongation, Elu, [%]—the elongation deter- generally necessary to use machined test specimens and to usemined at the maximum force sustained by the test piece just a special means of gripping to ensure that the specimens, whenprior to necking or fracture, or both. under load, shall be as nearly as possible in uniformly 18.104.22.168 Discussion—Uniform elongation includes both elas- distributed pure axial tension (see 5.2.3, 5.2.4, and 5.2.5).tic and plastic elongation. 5.2.3 Grips for Threaded and Shouldered Specimens and Brittle Materials—A schematic diagram of a gripping device4. Significance and Use for threaded-end specimens is shown in Fig. 3, while Fig. 4 4.1 Tension tests provide information on the strength and shows a device for gripping specimens with shouldered ends.ductility of materials under uniaxial tensile stresses. This Both of these gripping devices should be attached to the headsinformation may be useful in comparisons of materials, alloy of the testing machine through properly lubricated spherical-development, quality control, and design under certain circum- seated bearings. The distance between spherical bearingsstances. should be as great as feasible. 4.2 The results of tension tests of specimens machined to 5.2.4 Grips for Sheet Materials—The self-adjusting gripsstandardized dimensions from selected portions of a part or shown in Fig. 5 have proved satisfactory for testing sheetmaterial may not totally represent the strength and ductility materials that cannot be tested satisfactorily in the usual type ofproperties of the entire end product or its in-service behavior in wedge grips.different environments. 5.2.5 Grips for Wire—Grips of either the wedge or snub- 4.3 These test methods are considered satisfactory for ac- bing types as shown in Fig. 5 and Fig. 6 or flat wedge gripsceptance testing of commercial shipments. The test methods may be used.have been used extensively in the trade for this purpose. 5.3 Dimension-Measuring Devices—Micrometers and other devices used for measuring linear dimensions shall be accurate5. Apparatus and precise to at least one half the smallest unit to which the 5.1 Testing Machines—Machines used for tension testing individual dimension is required to be measured.shall conform to the requirements of Practices E 4. The forces 5.4 Extensometers—Extensometers used in tension testingused in determining tensile strength and yield strength shall be shall conform to the requirements of Practice E 83 for thewithin the verified force application range of the testing classifications specified by the procedure section of this testmachine as defined in Practices E 4. method. Extensometers shall be used and verified to include 5.2 Gripping Devices: strains corresponding to the yield strength and elongation at 5.2.1 General—Various types of gripping devices may be fracture (if determined).used to transmit the measured force applied by the testing 5.4.1 Extensometers with gage lengths equal to or shortermachine to the test specimens. To ensure axial tensile stress than the nominal gage length of the specimen (dimensionswithin the gage length, the axis of the test specimen should shown as ―G-Gage Length‖ in the accompanying figures) maycoincide with the center line of the heads of the testing be used to determine the yield behavior. For specimens withoutmachine. Any departure from this requirement may introduce a reduced section (for example, full cross sectional areabending stresses that are not included in the usual stress specimens of wire, rod, or bar), the extensometer gage lengthcomputation (force divided by cross-sectional area). for the determination of yield behavior shall not exceed 80 % NOTE 5—The effect of this eccentric force application may be of the distance between grips. For measuring elongation atillus- trated by calculating the bending moment and stress thus added. fracture with an appropriate extensometer the gage length ofFor a standard 12.5-mm diameter specimen, the stress increase is 1.5 % the extensometer shall be equal to the nominal gage lengthfor each required for the specimen being tested.0.025 mm of eccentricity. This error increases to about 2.5 %/0.025 mmfor a 9-mm diameter specimen and to about 3.2 %/0.025 mm for a 6-mm 6. Test Specimensdiameter specimen. 6.1 General: NOTE 6—Alignment methods are given in Practice E 1012. 6.1.1 Specimen Size—Test specimens shall be either sub- 5.2.2 Wedge Grips—Testing machines usually are equipped stantially full size or machined, as prescribed in the productwith wedge grips. These wedge grips generally furnish a specifications for the material being tested.satisfactory means of gripping long specimens of ductile metal 6.1.2 Location—Unless otherwise specified, the axis of theand flat plate test specimens such as those shown in Fig. 1. If, test specimen shall be located within the parent material ashowever, for any reason, one grip of a pair advances farther follows:than the other as the grips tighten, an undesirable bending 22.214.171.124 At the center for products 40 mm or less in thick-stress may be introduced. When liners are used behind the ness, diameter, or distance between flats.wedges, they must be of the same thickness and their faces 2
E 8M – 04 Di mensions, mm Standard Specimens Subsize Speci men Nominal Width Plate-Type Sheet-Type 6 mm 40 m m 12.5 mm G— Gage length (Note 1 and Note 2) 200.0 6 0.2 50.0 6 0.1 25.0 6 0.1 W— Width (Note 3 and Note 4) 40.0 6 2.0 12.5 6 0.2 6.0 6 0.1 T— Thickness (Note 5) thickness of material R— Radius of fillet, min (Note 6) 25 12.5 6 L— Overall length, (Note 2, Note 7 and Note 8) 450 200 100 A— Length of reduced section, min 225 57 32 B— Length of grip section, (Note 8) 75 50 30 C— Width of grip section, approximate (Note 4 and Note 9) 50 20 10 NOTE 1—For the 40-mm wide specimen, punch marks for measuring elongation after fracture shall be made on the flat or on the edge of the specimen and within the reduced section. Either a set of nine or more punch marks 25 mm apart, or one or more pairs of punch marks 200 mm apart, may be used. NOTE 2—When elongation measurements of 40-mm wide specimens are not required, a minimum length of reduced section (A) of 75 mm may be usedwith all other dimensions similar to the plate-type specimen. NOTE 3—For the three sizes of specimens, the ends of the reduced section shall not differ in width by more than 0.10, 0.05 or 0.02 mm, respectively.Also, there may be a gradual decrease in width from the ends to the center, but the width at each end shall not be more than 1 % larger than the widthat the center. NOTE 4—For each of the three sizes of specimens, narrower widths ( W and C) may be used when necessary. In such cases the width of the reducedsection should be as large as the width of the material being tested permits; however, unless stated specifically, the requirements for elongation in a productspecification shall not apply when these narrower specimens are used. NOTE 5—The dimension T is the thickness of the test specimen as provided for in the applicable material specifications. Minimum thickness of 40-mmwide specimens shall be 5 mm. Maximum thickness of 12.5-mm and 6-mm wide specimens shall be 19 mm and 6 mm, respectively. NOTE 6—For the 40-mm wide specimen, a 13-mm minimum radius at the ends of the reduced section is permitted for steel specimens under 690 MPain tensile strength when a profile cutter is used to machine the reduced section. NOTE 7—The dimension shown is suggested as a minimum. In determining the minimum length, the grips must not extend in to the transition sectionbetween Dimensions A and B, see Note 9. NOTE 8—To aid in obtaining axial force application during testing of 6-mm wide specimens, the overall length should be as large as the material willpermit, up to 200 mm. NOTE 9—It is desirable, if possible, to make the length of the grip section large enough to allow the specimen to extend into the grips a distance equalto two thirds or more of the length of the grips. If the thickness of 12.5-mm wide specimens is over 10 mm, longer grips and correspondingly longergrip sections of the specimen may be necessary to prevent failure in the grip section. NOTE 10—For the three sizes of specimens, the ends of the specimen shall be symmetrical in width with the center line of the reduced section within2.5, 0.25, and 0.13 mm, respectively. However, for referee testing and when required by product specifications, the ends of the 12.5-mm wide specimenshall be symmetrical within 0.2 mm. NOTE 11—For each specimen type, the radii of all fillets shall be equal to each other within a tolerance of 1.25 mm, and the centers of curvature ofthe two fillets at a particular end shall be located across from each other (on a line perpendicular to the centerline) within a tolerance of 2.5 mm. NOTE 12—Specimens with sides parallel throughout their length are permitted, except for referee testing, provided: (a) the above tolerances are used;(b) an adequate number of marks are provided for determination of elongation; and (c) when yield strength is determined, a suitable extensometer is used.If the fracture occurs at a distance of less than 2W from the edge of the gripping device, the tensile properties determined may not be representative ofthe material. In acceptance testing, if the properties meet the minimum requirements specified, no further testing is required, but if they are less than theminimum requirements, discard the test and retest. FIG. 1 Rectangular Tension Test Specimens 126.96.36.199 Midway from the center to the surface for productsover 40 mm in thickness, diameter, or distance between flats. 6.1.3 Specimen Machining—Improperly prepared testspecimens often are the reason for unsatisfactory and incorrecttest results. It is important, therefore, that care be exercised inthe preparation of specimens, particularly in the machining, tomaximize precision and minimize bias in test results. 188.8.131.52 The reduced sections of prepared specimens shouldbe free of cold work, notches, chatter marks, grooves, gouges, FIG. 2 Wedge Grips with Liners for Flat Specimens 3
E 8M – 04 FIG. 4 Gripping Device for Shouldered-End Specimens FIG. 3 Gripping Device for Threaded-End Specimensburrs, rough surfaces or edges, overheating, or any othercondition which may deleteriously affect the properties to bemeasured. NOTE 7—Punching or blanking of reduced section may producesig- nificant cold work or shear burrs, or both, along the edges whichshould be removed by machining. 184.108.40.206 Within the reduced section of rectangular speci-mens, edges or corners should not be ground or abraded in amanner which could cause the actual cross-sectional area of thespecimen to be significantly different from the calculated area. 220.127.116.11 For brittle materials, large radius fillets at the ends ofthe gage length should be used. 18.104.22.168 The cross-sectional area of the specimen should besmallest at the center of the reduced section to ensure fracturewithin the gage length. For this reason, a small taper ispermitted in the reduced section of each of the specimensdescribed in the following sections. 6.1.4 Specimen Surface Finish—When materials are testedwith surface conditions other than as manufactured, the surfacefinish of the test specimens shall be as provided in theapplicable product specifications. FIG. 5 Gripping Devices for Sheet and Wire Specimens NOTE 8—Particular attention should be given to the uniformityand quality of surface finish of specimens for high strength and verylow ductility materials, since this has been shown to be a factor in 6.2 Plate-Type Specimens—The standard plate-type speci-the variability of test results. men is shown in Fig. 1. This specimen is used for testing 4
E 8M – 04 6.3.2 Pin ends as shown in Fig. 7 may be used. In order to avoid buckling in tests of thin- and high-strength materials, it may be necessary to use stiffening plates at the grip ends. 6.4 Round Specimens: 6.4.1 The standard 12.5-mm diameter round test specimen shown in Fig. 8 is used quite generally for testing metallic materials, both cast and wrought. 6.4.2 Fig. 8 also shows small-size specimens proportional to the standard specimen. These may be used when it is necessary to test material from which the standard specimen or specimens shown in Fig. 1 cannot be prepared. Other sizes of small, round specimens may be used. In any such small-size specimen, it is important that the gage length for measurement of elongation FIG. 6 Snubbing Device for Testing Wire be five times the diameter of the specimen. 6.4.3 The shape of the ends of the specimen outside of themetallic materials in the form of plate, shapes, and flat material gage length shall be suitable to the material and of a shape tohaving a nominal thickness of 5 mm or over. When product fit the holders or grips of the testing machine so that the forcesspecifications so permit, other types of specimens may be used, may be applied axially. Fig. 9 shows specimens with variousas provided in 6.3, 6.4, and 6.5. types of ends that have given satisfactory results. 6.3 Sheet-Type Specimens: 6.5 Specimens for Sheet, Strip, Flat Wire, and Plate—In 6.3.1 The standard sheet-type test specimen is shown in Fig. testing sheet, strip, flat wire, and plate, use a specimen type1. This specimen is used for testing metallic materials in the appropriate for the nominal thickness of the material, asform of sheet, plate, flat wire, strip, band, hoop, rectangles, and described in the following:shapes ranging in nominal thickness from 0.13 to 19 mm. 6.5.1 For material with a nominal thickness of 0.13 - 5 mm,When product specifications so permit, other types of speci- use the sheet-type specimen described in 6.3.mens may be used as provided in 6.2, 6.4, and 6.5. 6.5.2 For material with a nominal thickness of 5 - 12.5 mm, NOTE 9—Test Methods E 345 may be used for tension testing use either the sheet-type specimen of 6.3 or the plate-typeof materials in thicknesses up to 0.150 mm. specimen of 6.2. Dimensions, mm G— Gage length 50.0 6 0.1 W— Width (Note 1) 12.5 6 0.2 T— Thickness, max (Note 2) 12.5 R— Radius of fillet, min (Note 3) 13 L— Overall length, min 200 A— Length of reduced section, min 57 B— Length of grip section, min 50 C— Width of grip section, approximate 50 D— Diameter of hole for pin, min (Note 4) 13 E— Edge distance from pin, approximate 40 F— Distance from hole to fillet, min 15 NOTE 1—The ends of the reduced section shall differ in width by not more than 0.1 mm. There may be a gradual taper in width from the ends to thecenter, but the width at each end shall be not more than 1 % greater than the width at the center. NOTE 2—The dimension T is the thickness of the test specimen as stated in the applicable product specifications. NOTE 3—For some materials, a fillet radius R larger than 13 mm may be needed. NOTE 4—Holes must be on center line of reduced section, within 6 0.1 mm. NOTE 5—Variations of dimensions C, D, E, F, and L may be used that will permit failure within the gage length. FIG. 7 Pin-Loaded Tension Test Specimen with 50-mm Gage Length 5
E 8M – 04 Di mensions, mm Standard Specimen S all-Size Specimens Proportional To Standard 12.5 9 6 4 2.5 G—Gage length 62.5 6 0.1 45.06 0.1 30.0 6 0.1 20.06 0.1 12.5 6 0.1 D—Diameter (Note 1) 12.5 6 0.2 9.0 6 0.1 6.0 6 0.1 4.0 6 0.1 2.5 6 0.1 R—Radius of fillet, min 10 8 6 4 2 A—Length of reduced section, min (Note 2) 75 54 36 24 20 NOTE 1—The reduced section may have a gradual taper from the ends toward the center, with the ends not more than 1 % larger in diameter than thecenter (controlling dimension). NOTE 2—If desired, the length of the reduced section may be increased to accommodate an extensometer of any convenient gage length. Referencemarks for the measurement of elongation should, nevertheless, be spaced at the indicated gage length. NOTE 3—The gage length and fillets shall be as shown, but the ends may be of any form to fit the holders of the testing machine in such a way thatthe load may be axial (see Fig. 9). If the ends are to be held in wedge grips it is desirable, if possible, to make the length of the grip section great enoughto allow the specimen to extend into the grips a distance equal to two thirds or more of the length of the grips. NOTE 4—On the round specimens in Figs. 8 and 9, the gage lengths are equal to five times the nominal diameter. In some product specifications otherspecimens may be provided for, but the 5-to-1 ratio is maintained within dimensional tolerances, the elongation values may not be comparable with thoseobtained from the standard test specimen. NOTE 5—The use of specimens smaller than 6 mm in diameter shall be restricted to cases when the material to be tested is of insufficient size to obtainlarger specimens or when all parties agree to their use for acceptance testing. Smaller specimens require suitable equipment and greater skill in bothmachining and testing.FIG. 8 Standard 12.5-mm Round Tension Test Specimen with Gage Lengths Five Times the Diameters (5D), and Examples of Small-Size Specimens Proportional to the Standard Specimen 6.5.3 For material with a nominal thickness of 12.5 - 19 22.214.171.124 Full Cross Section (Note 10)—It is permissible tomm, use either the sheet-type specimen of 6.3, the plate-type reduce the test section slightly with abrasive cloth or paper, orspecimen of 6.2, or the largest practical size of round specimen machine it sufficiently to ensure fracture within the gagedescribed in 6.4. marks. For material not exceeding 5 mm in diameter or 6.5.4 For material with a nominal thickness of 19 mm, or distance between flats, the cross-sectional area may be reducedgreater, use the plate-type specimen of paragraph 6.2 or the to not less than 90 % of the original area without changing thelargest practical size of round specimen described in 6.4. shape of the cross section. For material over 5 mm in diameter 126.96.36.199 If the product specifications permit, material of a or distance between flats, the diameter or distance between flatsthickness of 19 mm or greater may be tested using a modified may be reduced by not more than 0.25 mm without changingsheet-type specimen conforming to the configuration shown by the shape of the cross section. Square, hexagonal, or octagonalFig. 1. The thickness of this modified specimen must be wire or rod not exceeding 5 mm between flats may be turnedmachined to 10 +/- 0.50 mm and must be uniform within 0.1 to a round having a cross-sectional area not smaller than 90 %mm throughout the reduced section. In the event of disagree- of the area of the maximum inscribed circle. Fillets, preferablyment, a round specimen shall be used as the referee specimen. with a radius of 10 mm, but not less than 3 mm, shall be used 6.6 Specimens for Wire, Rod, and Bar: at the ends of the reduced sections. Square, hexagonal, or 6.6.1 For round wire, rod, and bar, test specimens having the octagonal rod over 5 mm between flats may be turned to afull cross-sectional area of the wire, rod, or bar shall be used round having a diameter no smaller than 0.25 mm less than thewherever practicable. The gage length for the measurement of original distance between flats.elongation of wire less than 4 mm in diameter shall be asprescribed in product specifications. In testing wire, rod, or bar NOTE 10—The ends of copper or copper alloy specimens maythat has a 4 mm or larger diameter, unless otherwise specified, be flattened 10 to 50 % from the original dimension in a jig similar toa gage length equal to five times the diameter shall be used. that shown in Fig. 10, to facilitate fracture within the gage marks. In flattening the opposite ends of the test specimen, care shall be taken toThe total length of the specimens shall be at least equal to the ensure that the four flattened surfaces are parallel and that the two parallelgage length plus the length of material required for the full use surfaces on the same side of the axis of the test specimen lie in the sameof the grips employed. plane. 6.6.2 For wire of octagonal, hexagonal, or square crosssection, for rod or bar of round cross section where the 188.8.131.52 For rod and bar, the largest practical size of roundspecimen required in 6.6.1 is not practicable, and for rod or bar specimen as described in 6.4 may be used in place of a testof octagonal, hexagonal, or square cross section, one of the specimen of full cross section. Unless otherwise specified infollowing types of specimens shall be used: the product specification, specimens shall be parallel to the direction of rolling or extrusion. 6
E 8M – 04 Dimensions, mm Specimen 1 Specimen 2 Specimen 3 Specimen 4 Specimen 5 G—Gage length 62.5 6 0.1 62.56 0.1 62.5 6 0.1 62.5 6 0.1 62.5 6 0.1 D—Diameter (Note 1) 12.5 6 0.2 12.5 6 0.2 12.5 6 0.2 12.56 0.2 12.5 6 0.2 R—Radius of fillet, min 10 10 2 10 10 A—Length of reduced section 75, min 75, min 100, approxi mately 75, min 75, min L—Overall length, approximate 145 155 140 140 255 B—Length of end section (Note 3) 35, approxi mately 25, approximately 20, approxi mately 15, approximately 75, min C—Diameter of end section 20 20 20 22 20 E—Length of shoulder and fillet ... . 15 ... . 20 15 section, approximate F—Diameter of shoulder ... . 15 ... . 15 15 NOTE 1—The reduced section may have a gradual taper from the ends toward the center with the ends not more than 1 % larger in diameter than thecenter. NOTE 2—On Specimens 1 and 2, any standard thread is permissible that provides for proper alignment and aids in assuring that the specimen will breakwithin the reduced section. NOTE 3—On Specimen 5 it is desirable, if possible, to make the length of the grip section great enough to allow the specimen to extend into the gripsa distance equal to two thirds or more of the length of the grips. FIG. 9 Various Types of Ends for Standard Round Tension Test Specimens 6.7.2 Rectangular bars of thickness small enough to fit the grips of the testing machine but of too great width may be reduced in width by cutting to fit the grips, after which the cut surfaces shall be machined or cut and smoothed to ensure failure within the desired section. The reduced width shall be not less than the original bar thickness. Also, one of the types of specimens described in 6.2, 6.3, and 6.4 may be used. 6.8 Shapes, Structural and Other—In testing shapes other than those covered by the preceding sections, one of the types of specimens described in 6.2, 6.3, and 6.4 shall be used. 6.9 Specimens for Pipe and Tube (Note 11): 6.9.1 For all small tube (Note 11), particularly sizes 25 mm and under in nominal outside diameter, and frequently for larger sizes, except as limited by the testing equipment, it is FIG. 10 Squeezing Jig for Flattening Ends of Full-Size Tension standard practice to use tension test specimens of full-size Test Specimens tubular sections. Snug-fitting metal plugs shall be inserted far enough into the ends of such tubular specimens to permit the 6.7 Specimens for Rectangular Bar— In testing rectangular testing machine jaws to grip the specimens properly. The plugsbar one of the following types of specimens shall be used: shall not extend into that part of the specimen on which the 6.7.1 Full Cross Section—It is permissible to reduce the elongation is measured. Elongation is measured over a lengthwidth of the specimen throughout the test section with abrasive of 5D unless otherwise stated in the product specification. Fig.cloth or paper, or by machining sufficiently to facilitate fracture 11 shows a suitable form of plug, the location of the plugs inwithin the gage marks, but in no case shall the reduced width the specimen, and the location of the specimen in the grips ofbe less than 90 % of the original. The edges of the midlength the testing machine.of the reduced section not less than 20 mm in length shall beparallel to each other and to the longitudinal axis of the NOTE 11—The term ―tube‖ is used to indicate tubular products in general, and includes pipe, tube, and tubing.specimen within 0.05 mm. Fillets, preferably with a radius of10 mm but not less than 3 mm, shall be used at the ends of the 6.9.2 For large-diameter tube that cannot be tested in fullreduced sections. section, longitudinal tension test specimens shall be cut as 7
E 8M – 04 form and dimensions shown for Specimen 2 in Fig. 13. When using the latter specimen, either or both surfaces of the specimen may be machined to secure a uniform thickness, provided not more than 15 % of the normal wall thickness is removed from each surface. For large tube 20 mm and over in wall thickness, the standard specimen shown in Fig. 8 shall be used for transverse tension tests. Specimens for transverse tension tests on large welded tube to determine the strength of welds shall be located perpendicular to the welded seams, with the welds at about the middle of their lengths. 6.10 Specimens for Forgings—For testing forgings, the largest round specimen described in 6.4 shall be used. If round specimens are not feasible, then the largest specimen described in 6.5 shall be used. 6.10.1 For forgings, specimens shall be taken as provided in NOTE 1—The diameter of the plug shall have a slight taper from the the applicable product specifications, either from the predomi-line limiting the testing machine jaws to the curved section. nant or thickest part of the forging from which a coupon can be FIG. 11 Metal Plugs for Testing Tubular Specimens, Proper Location of Plugs in Specimen and of Specimen in Heads of obtained, or from a prolongation of the forging, or from Testing Machine separately forged coupons representative of the forging. When not otherwise specified, the axis of the specimen shall be parallel to the direction of grain flow.indicated in Fig. 12. Specimens from welded tube shall be 6.11 Specimens for Castings—In testing castings either thelocated approximately 90° from the weld. If the tube-wall standard specimen shown in Fig. 8 or the specimen shown inthickness is under 20 mm, either a specimen of the form and Fig. 15 shall be used unless otherwise provided in the productdimensions shown in Fig. 13 or one of the small-size speci- specifications.mens proportional to the standard 12.5-mm specimen, as 6.11.1 Test coupons for castings shall be made as shown inmentioned in 6.4.2 and shown in Fig. 8, shall be used. Fig. 16 and Table 1.Specimens of the type shown in Fig. 13 may be tested with 6.12 Specimen for Malleable Iron—For testing malleablegrips having a surface contour corresponding to the curvature iron the test specimen shown in Fig. 17 shall be used, unlessof the tube. When grips with curved faces are not available, the otherwise provided in the product specifications.ends of the specimens may be flattened without heating. If the 6.13 Specimen for Die Castings—For testing die castingstube-wall thickness is 20 mm or over, the standard specimen the test specimen shown in Fig. 18 shall be used unlessshown in Fig. 8 shall be used. otherwise provided in the product specifications. NOTE 12—In clamping of specimens from pipe and tube (as may 6.14 Specimens for Powder Metallurgy (P/M) Materials—be done during machining) or in flattening specimen ends (for gripping), For testing powder metallurgy (P/M) materials the test speci-care must be taken so as not to subject the reduced section to any mens shown in Fig. 19 and Fig. 20 shall be used, unlessdeformation or cold work, as this would alter the mechanical properties. otherwise provided in the product specifications. When making 6.9.3 Transverse tension test specimens for tube may be test specimens in accordance with Fig. 19, shallow transversetaken from rings cut from the ends of the tube as shown in Fig. grooves, or ridges, may be pressed in the ends to allow14. Flattening of the specimen may be either after separating as gripping by jaws machined to fit the grooves or ridges. Becausein A, or before separating as in B. Transverse tension test of shape and other factors, the flat unmachined tensile testspecimens for large tube under 20 mm in wall thickness shall specimen (Fig. 19) in the heat-treated condition will have anbe either of the small-size specimens shown in Fig. 8 or of the ultimate tensile strength of 50 % to 85 % of that determined in a machined round tensile test specimen (Fig. 20) of like composition and processing. 7. Procedures 7.1 Preparation of the Test Machine— Upon startup or following a prolonged period of machine inactivity, the test machine should be exercised or warmed up to normal operating temperatures to minimize errors that may result from transient conditions. 7.2 Measurement of Dimensions of Test Specimens: 7.2.1 To determine the cross-sectional area of a test speci- men, measure the dimensions of the cross section at the center NOTE 1—The edges of the blank for the specimen shall be cut of the reduced section. For referee testing of specimens underparallel to each other. 5 mm in their least dimension, measure the dimensions where FIG. 12 Location from Which Longitudinal Tension Test the least cross-sectional area is found. Measure and record the Specimens Are to Be Cut from Large-Diameter Tube cross-sectional dimensions of tension test specimens 5 mm and 8
E 8M – 04 Di mensions, mm Specimen 1 Specimen 2 Specimen 3 Specimen 4 Specimen 5 Specimen 6 Specimen 7 Nominal Width 12.5 40 40 20 20 25 25 G—Gage length 50.0 6 0.1 50.0 6 0.1 200.0 6 0.2 50.0 6 0.1 100.0 6 0.1 50.0 6 0.1 100.0 6 0.1 W—Width (Note 1) 12.5 6 0.2 40.06 2.0 40.0 6 2.0 20.0 6 0.7 20.0 6 0.7 25.0 6 1.5 25.0 6 1.5 T—Thickness measured thickness of specimen R—Radius of fillet, min 12.5 25 25 25 25 25 25 A—Length of reduced section, min 60 60 230 60 120 60 120 B—Length of grip section, min (Note 2) 75 75 75 75 75 75 75 C—Width of grip section, approximate (Note 3) 20 50 50 25 25 40 40 NOTE 1—The ends of the reduced section shall not differ in width by more than 0.1 mm for specimens 1–7. There may be a gradual taper in widthfrom the ends to the center, but the width at each end shall be not more than 1 % greater than the width at the center. NOTE 2—It is desirable, if possible, to make the length of the grip section great enough to allow the specimen to extend into the grips a distance equalto two thirds or more of the length of the grips. NOTE 3—The ends of the specimen shall be symmetrical with the center line of the reduced section within 1.0 mm for specimens 1, 4, and 5 and 2.5mm for specimens 2, 3, 6, and 7. NOTE 4—For circular segments, the cross-sectional area may be calculated by multiplying W and T. If the ratio of the dimension W to the diameterof the tubular section is larger than about 1⁄6 , the error in using this method to calculate cross-sectional area may be appreciable. In this case, the exactequaton (see 7.3.2) must be used to determine the area. NOTE 5—For each specimen type, the radii of all fillets shall be equal to each other within a tolerance of 1.25 mm, and the centers of curvature of thetwo fillets at a particular end shall be located across from each other (on a line perpendicular to the centerline) within a tolerance of 2.5 mm. NOTE 6—Specimens with sides parallel throughout their length are permitted, except for referee testing and where prohibited by product specification,provided: (a) the above tolerances are used; (b) an adequate number of marks are provided for determination of elongation; and (c) when yield strengthis determined, a suitable extensometer is used. If the fracture occurs at a distance of less than 2W from the edge of the gripping device, the tensileproperties determined may not be representative of the material. If the properties meet the minimum requirements specified, no further testing is required,but if they are less than the minimum requirements, discard the test and retest. FIG. 13 Tension Test Specimens for Large-Diameter Tubular Products determining the mass of a length not less than 20 times longer than the largest cross-sectional dimension. 184.108.40.206 Determine the weight to the nearest 0.5 % or less. 220.127.116.11 The cross-sectional area is equal to the mass of the specimen divided by the length and divided by the density of FIG. 14 Location of Transverse Tension Test Specimen in Ring the material. Cut from Tubular Products 7.2.3 When using specimens of the type shown in Fig. 13over to the nearest 0.02 mm; the cross-sectional dimensions taken from tubes, the cross-sectional area shall be determinedless than 5 mm and not less than 2.5 mm to the nearest 0.01 as follows:mm; the cross-sectional dimensions less than 2.5 mm and not If D/W # 6:less than 0.50 mm to the nearest 0.002 mm; and when practical, A 5 [~ W/4 ! 3 ~ D 2 2 W 2!1 / 2# 1 [ ~D 2/4 !the cross-sectional dimensions less than 0.50 mm to at least the 3 arcsin ~W/D !# 2 [ ~ W/4 ! 3 ~~ D 2 2T! 2 2 W 2!1 / 2#nearest 1 % but in all cases to at least the nearest 0.002 mm. 2 [~~ D 2 2T!/2 ! 2 3 arcsin ~W/~ D 2 2T !!# NOTE 13—Accurate and precise measurement of specimen (1)dimensions can be one of the most critical aspects of tension testing,depending on specimen geometry. See Appendix X2 for additional where:information. NOTE 14—Rough surfaces due to the manufacturing process such as A = exact cross-sectional area, mm2, hot rolling, metallic coating, etc., may lead to inaccuracy of the W = width of the specimen in the reduced section, mm, computed areas greater than the measured dimensions would indicate. D = measured outside diameter of the tube, mm, and Therefore, cross-sectional dimensions of tension test specimens with T = measured wall thickness of the specimen, mm. rough surfaces due to processing may be measured and recorded to the nearest 0.02 mm. NOTE 15—See X2.9 for cautionary information on arcsin values to be in radians measurements taken If D/W > 6, the exact equation or the following equation mayfrom coated metal products. be used: 7.2.2 Determine the cross-sectional area of a full-size test A5W3T (2)specimen of uniform but nonsymmetrical cross section by
E 8M – 04 Dimensions, mm Specimen 1 Specimen 2 Specimen 3 Nominal Diameter 12.5 20 30 G—Length of parallel Shall be equal to or greater than diameter D D—Diameter 12.5 6 0.2 20.0 6 0.4 30.0 6 0.6 R—Radius of fillet, min 25 25 50 A—Length of reduced section, min 32 38 60 L—Overall length, min 95 100 160 B—Length of end section, approximate 25 25 45 C—Diameter of end section, approximate 20 30 48 E—Length of shoulder, min 6 6 8 F—Diameter of shoulder 16.0 6 0.4 24.06 0.4 36.5 6 0.4 NOTE 1—The reduced section and shoulders (dimensions A, D, E, F, G, and R) shall be as shown, but the ends may be of any form to fit the holdersof the testing machine in such a way that the force shall be axial. Commonly the ends are threaded and have the dimensions B and C given above. FIG. 15 Standard Tension Test Specimen for Cast Iron (a) Design for Double Keel Block Coupon (b) Design for Multiple Keel Block Coupon (4 Legs) (c) Design for ―Attached‖ Coupon FIG. 16 Test Coupons for Castings (see Table 1 for Details of Design) 10
E 8M – 04 TABLE 1 Details of Test Coupon Design for Castings (See Fig. 16) NOTE 1—Test Coupons for Large and Heavy Steel Castings: The test coupons in Fig. 16 are to be used for large and heavy steel castings. However,at the option of the foundry the cross-sectional area and length of the standard coupon may be increased as desired. This provision does not apply toSpecification A 356/A 356M. NOTE 2—Bend Bar: If a bend bar is required, an alternate design (as shown by dotted lines in Fig. 16) is indicated. Log Design (125 mm) Ri ser Design1. L (length) A 125-mm minimum length will be used. This length 1. L (length) The length of the riser at the base will be the same as may be increased at the option of the foundry to ac- the top length of the leg. The length of the riser at the commodate additional test bars (see Note 1). top therefore depends on the amount of taper added to the riser.2. End taper Use of and size of end taper is at the option of the 2. Width The width of the riser at the base of a multiple-leg cou- foundry. pon shall be n (57 mm) − 16 mm where n equals the number of legs attached to the coupon. The width of the riser at the top is therefore dependent on the amount of taper added to the riser.3. Height 32 mm4. Width (at top) 32 mm (see Note 1).5. Radius (at bottom) 13 mm max6. Spacing between legs A 13-mm radius will be used between the legs.7. Location of test bars The tensile, bend, and impact bars will be taken from the lower portion of the leg (see Note 2).8. Number of legs The number of legs attached to the coupon is at the 3. T (riser Use of and size is at the option of the foundry. option of the foundry providing they are equispaced taper) The minimum height of the riser shall be 51 mm. The according to Item 6. Height maximum height is at the option of the foundry for the following reasons: (a) many risers are cast open, (b) different compositions may require variation in risering for soundness, or (c) different pouring temperatures may require variation in risering for soundness.9. Rs Radius from 0 to approximately 2 mm Dimensions, mm D—Diameter 16 R—Radius of fillet 8 A—Length of reduced section 64 L—Overall length 190 B—Length of end section 64 C—Diameter of end section 20 E—Length of fillet 5 FIG. 17 Standard Tension Test Specimen for Malleable Iron where: 7.3.2 For materials where the specified elongation is 3 % or A = approximate cross-sectional area, mm2, less, measure the original gage length to the nearest 0.05 mm W = width of the specimen in the reduced section, mm, prior to testing. and 7.4 Zeroing of the Testing Machine: T = measured wall thickness of the specimen, mm. 7.4.1 The testing machine shall be set up in such a manner NOTE 16—See X2.8 for cautionary information on measurements and that zero force indication signifies a state of zero force on thecalculations for specimens taken from large-diameter tubing. specimen. Any force (or preload) imparted by the gripping of 7.3 Gage Length Marking of Test Specimens: the specimen (see Note 17) must be indicated by the force 7.3.1 The gage length for the determination of elongation measuring system unless the preload is physically removedshall be in accordance with the product specifications for the prior to testing. Artificial methods of removing the preload onmaterial being tested. Gage marks shall be stamped lightly with the specimen, such as taring it out by a zero adjust pot ora punch, scribed lightly with dividers or drawn with ink as removing it mathematically by software, are prohibited be-preferred. For material that is sensitive to the effect of slight cause these would affect the accuracy of the test results.notches and for small specimens, the use of layout ink will aidin locating the original gage marks after fracture. 11
E 8M – 04 Di mensions, mmG—Gage length 50.0 6 0.1D—Diameter (see Note) 6.4 6 0.1 Approximate Pressing Area of Unmachined Compact = 752 m m 2R—Radius of fillet, min 75 Machining RecommendationsA—Length of reduced section, min 60 1. Rough machine reduced section to 6.35 mm diameterL—Overall length, min 230 2. Finish turn 4.75/4.85 mm diameter with radii and taperB—Distance between grips, min 115 3. Polish with 00 emery clothC—Diameter of end section, approximate 10 4. Lap with crocus cloth Di mensions, mm NOTE 1—The reduced section may have a gradual taper from the ends G—Gage length 25.40 6 0.8toward the center, with the ends not more than 0.1 mm larger in diameter D—Diameter at center of reduced section 4.756 0.03than the center. H—Diameter at ends of gage length 4.856 0.03 FIG. 18 Standard Tension Test Specimen for Die Castings R—Radius of fillet 6.35 6 0.13 A—Length of reduced section 47.63 6 0.13 L—Overall length (die cavity length) 75, nominal B—Length of end section 7.88 6 0.13 C—Compact to this end thickness 10.03 6 0.13 W—Die cavity width 10.03 6 0.08 E—Length of shoulder 6.35 6 0.13 F—Diameter of shoulder 7.88 6 0.03 J—End fillet radius 1.27 6 0.13 NOTE 1—The gage length and fillets of the specimen shall be as shown. The ends as shown are designed to provide a practical minimum Pressing Area = 645 mm2 pressing area. Other end designs are acceptable, and in some cases are NOTE 1—Dimensions specified, except G and T, are those of the die. required for high-strength sintered materials. NOTE 2—It is recommended that the test specimen be gripped with Dimensions, mm a split collet and supported under the shoulders. The radius of the colletG—Gage length 25.40 6 0.8 support circular edge is to be not less than the end fillet radius of the testD—Width at center 5.72 6 0.03 specimen.W—Width at end of reduced section 5.97 6 0.03 NOTE 3—Diameters D and H are to be concentric within 0.03 mm totalT—Compact to this thickness 3.56 to 6.35 indicator runout (T.I.R.), and free of scratches and tool marks.R—Radius of fillet 25.4A—Half-length of reduced section 15.88 FIG. 20 Standard Round Machined Tension Test Specimen forB—Grip length 80.95 6 0.03 Powder Metallurgy (P/M) ProductsL—Overall length 89.64 6 0.03C—Width of grip section 8.71 6 0.03F—Half-width of grip section 4.34 6 0.03 7.6 Speed of Testing:E—End radius 4.34 6 0.03 7.6.1 Speed of testing may be defined in terms of (a) rate of FIG. 19 Standard Flat Unmachined Tension Test Specimen for straining of the specimen, ( b) rate of stressing of the specimen, Powder Metallurgy (P/M) Products (c) rate of separation of the two heads of the testing machine during a test, (d) the elapsed time for completing part or all of the test, or (e) free-running crosshead speed (rate of movement NOTE 17—Preloads generated by gripping of specimens may be of the crosshead of the testing machine when not under load).either tensile or compressive in nature and may be the result of such 7.6.2 Specifying suitable numerical limits for speed andthings as: — grip design selection of the method are the responsibilities of the product — malfunction of gripping apparatus (sticking, binding, etc.) committees. Suitable limits for speed of testing should be — excessive gripping force specified for materials for which the differences resulting from — sensitivity of the control loop the use of different speeds are of such magnitude that the test NOTE 18—It is the operator’s responsibility to verify that an observed results are unsatisfactory for determining the acceptability ofpreload is acceptable and to ensure that grips operate in a smooth manner. the material. In such instances, depending upon the materialUnless otherwise specified, it is recommended that momentary (dynamic)forces due to gripping not exceed 20 % of the material’s nominal yield and the use for which the test results are intended, one or morestrength and that static preloads not exceed 10 % of the material’s nominal of the methods described in the following paragraphs isyield strength. recommended for specifying speed of testing. 7.5 Gripping of the Test Specimen: NOTE 19—Speed of testing can affect test values because of the 7.5.1 For specimens with reduced sections, gripping of the rate sensitivity of materials and the temperature-time effects.specimen shall be restricted to the grip section, because 18.104.22.168 Rate of Straining—The allowable limits for rate ofgripping in the reduced section or in the fillet can significantly straining shall be specified in metres per metre per second.affect test results.
E 8M – 04Some testing machines are equipped with pacing or indicating 22.214.171.124 The speed of testing shall be such that the forces anddevices for the measurement and control of rate of straining, strains used in obtaining the test results are accurately indi-but in the absence of such a device the average rate of straining cated.can be determined with a timing device by observing the time 126.96.36.199 When performing a test to determine yield proper-required to effect a known increment of strain. ties, the rate of stress application shall be between 1.15 and 188.8.131.52 Rate of Stressing—The allowable limits for rate of 11.5 MPa/s.stressing shall be specified in megapascals per second. Many NOTE 22—When a specimen being tested begins to yield, thetesting machines are equipped with pacing or indicating stressing rate decreases and may even become negative in the case of adevices for the measurement and control of the rate of specimen with discontinuous yielding. To maintain a constant stressingstressing, but in the absence of such a device the average rate rate in this case would require the testing machine to operate at extremelyof stressing can be determined with a timing device by high speeds and, in many cases, this is not practical. The speed of theobserving the time required to apply a known increment of testing machine shall not be increased in order to maintain a stressing rate when the specimen begins to yield. In practice, it isstress. simpler to use either a strain rate, a rate of separation of the heads, or a 184.108.40.206 Rate of Separation of Heads During Tests—The free-running crosshead speed which approximates the desired stressingallowable limits for rate of separation of the heads of the rate. As an example, use a strain rate that is less than 11.5 MPa/s dividedtesting machine, during a test, shall be specified in metres per by the nominal Young’s Modulus of the material being tested. As anothermetre of length of reduced section (or distance between grips example, find a rate of separation of the heads throughfor specimens not having reduced sections) per second. The experimentation which would approximate the desired stressing ratelimits for the rate of separation may be further qualified by prior to the onset of yielding, and maintain that rate of separation of the heads through the region that yield properties are determined. Whilespecifying different limits for various types and sizes of both of these methods will provide similar rates of stressing andspecimens. Many testing machines are equipped with pacing or straining prior to the onset of yielding, the rates of stressing and strainingindicating devices for the measurement and control of the rate may be different in the region where yield properties are determined.of separation of the heads of the machine during a test, but in This difference is due to the change in the rate of elasticthe absence of such a device the average rate of separation of deformation of the testing machine, before and after the onset of yielding.the heads can be experimentally determined by using suitable In addition, the use of any of the methods other than rate of straining may result in different stressing and straining rates when using different testinglength-measuring and timing devices. machines, due to differences in the stiffness of the testing machines used. 220.127.116.11 Elapsed Time—The allowable limits for the elapsedtime from the beginning of force application (or from some 7.6.4 Speed of Testing When Determining Tensilespecified stress) to the instant of fracture, to the maximum Strength—In the absence of any specified limitations on speedforce, or to some other stated stress, shall be specified in of testing, the following general rules shall apply for materialsminutes or seconds. The elapsed time can be determined with with expected elongations greater than 5 %. When determininga timing device. only the tensile strength, or after the yield behavior has been 18.104.22.168 Free-Running Crosshead Speed—The allowable recorded, the speed of the testing machine shall be set betweenlimits for the rate of movement of the crosshead of the testing 0.05 and 0.5 m/m of the length of the reduced section (ormachine, with no force applied by the testing machine, shall be distance between the grips for specimens not having reducedspecified in metres per metre of length of reduced section (or sections) per minute. Alternatively, an extensometer and straindistance between grips for specimens not having reduced rate indicator may be used to set the strain between 0.05 andsections) per second. The limits for the crosshead speed may be 0.5 m/m/min.further qualified by specifying different limits for various types NOTE 23—For materials with expected elongations less than or equal toand sizes of specimens. The average crosshead speed can be 5 %, the speed of the testing machine may be maintained throughout theexperimentally determined by using suitable length-measuring test at the speed used to determine yield properties.and timing devices. NOTE 24—Tensile strength and elongation are sensitive to test speed for many materials (see Appendix XI) to the extent that variations within NOTE 20—For machines not having crossheads or having the range of test speeds given above can significantly affect results.stationary crossheads, the phrase ―free-running crosshead speed‖ may beinterpreted to mean the free-running rate of grip separation. 7.7 Determination of Yield Strength—Determine yield 7.6.3 Speed of Testing When Determining Yield strength by any of the methods described in 7.7.1 to 7.7.4.Properties—Unless otherwise specified, any convenient speed Where extensometers are employed, use only those which areof testing may be used up to one half the specified yield verified over a strain range in which the yield strength will bestrength or up to one quarter the specified tensile strength, determined (see 5.4).whichever is smaller. The speed above this point shall be NOTE 25—For example, a verified strain range of 0.2 to 2.0 %within the limits specified. If different speed limitations are is appropriate for use in determining the yield strengths of many metals.required for use in determining yield strength, yield point NOTE 26—Determination of yield behavior on materials which cannotelongation, tensile strength, elongation, and reduction of area, support an appropriate extensometer (thin wire, for example) is problem- atic and outside the scope of this standard.they should be stated in the product specifications. In theabsence of any specified limitations on speed of testing, the 7.7.1 Offset Method—To determine the yield strength by thefollowing general rules shall apply: offset method, it is necessary to secure data (autographic or NOTE 21—In the previous and following paragraphs, the yield numerical) from which a stress-strain diagram may be drawn.proper- ties referred to include yield strength and yield point elongation. Then on the stress-strain diagram (Fig. 21) lay off Om equal to the specified value of the offset, draw mn parallel to OA, and 13
E 8M – 04 FIG. 22 Stress-Strain Diagram for Determination of Yield Strength by the Extension-Under-Load Method measurement of YPE if observed. If Class C devices are used,FIG. 21 Stress-Strain Diagram for Determination of Yield Strength this must be reported along with the results. by the Offset Method NOTE 29—The appropriate value of the total extension must be speci- fied. For steels with nominal yield strengths of less than 550 MPa, an appropriate value is 0.005 mm/mm (0.5 %) of the gage length.thus locate r, the intersection of mn with the stress-strain For higher strength steels, a greater extension or the offset methoddiagram (Note 32). In reporting values of yield strength should be used. NOTE 30—When no other means of measuring elongationobtained by this method, the specified value of offset used are available, a pair of dividers or similar device can be used to determine a point ofshould be stated in parentheses after the term yield strength, as detectable elongation between two gage marks on the specimen. The gagefollows: length shall be 50 mm. The stress corresponding to the load at the instant yield strength ~offset 5 0.2 %! 5 360 MPa (3) of detectable elongation may be recorded as the approximate extension- under-load yield strength. In using this method, a Class B2 or better extensometer (seePractice E 83) shall be used. 7.7.3 Autographic Diagram Method (for materials exhibit- ing discontinuous yielding)—Obtain stress-strain (or force- NOTE 27—There are two general types of extensometers, averaging elongation) data or construct a stress-strain (or load-and non-averaging, the use of which is dependent on the product tested.For most machined specimens, there are minimal differences. elongation) diagram using an autographic device. DetermineHowever, for some forgings and tube sections, significant differences in the upper or lower yield strength as follows:measured yield strength can occur. For these cases, it is recommended 22.214.171.124 Record the stress corresponding to the maximumthat the averaging type be used. force at the onset of discontinuous yielding as the upper yield NOTE 28—When there is a disagreement over yield properties, strength. This is illustrated in Fig. 23 and Fig. 24.the offset method for determining yield strength is recommended asthe referee method. NOTE 31—If multiple peaks are observed at the onset of discontinuous yielding, the first is considered the upper yield strength. 7.7.2 Extension-Under-Load Method—Yield strength by the (See Fig. 24.)extension-under-load method may be determined by: ( 1) usingautographic or numerical devices to secure stress-strain data, 126.96.36.199 Record the minimum stress observed during discon- tinuous yielding (ignoring transient effects) as the lower yieldand then analyzing this data (graphically or using automatedmethods) to determine the stress value at the specified value of strength. This is illustrated in Fig. 24.extension, or ( 2) using devices that indicate when the specified NOTE 32—Yield properties of materials exhibiting yield pointextension occurs, so that the stress then occurring may be elonga- tion are often less repeatable and less reproducible than those ofascertained (Note 30). Any of these devices may be automatic. similar materials having no YPE. Offset and EUL yield strengths may be significantly affected by force fluctuations occurring in theThis method is illustrated in Fig. 22. The stress at the specified region where the offset or extension intersects the stress-strain curve.extension shall be reported as follows: Determination of upper or lower yield strengths (or both) may therefore yield strength ~EUL 5 0.5 %! 5 360 MPa (4) be preferable for such materials, although these properties are dependent on variables such as test machine stiffness and alignment. Speed of Extensometers and other devices used in determination of testing may also have a significant effect, regardless of the methodthe extension shall meet Class B2 requirements (see Practice employed.E 83) at the strain of interest, except where use of low- NOTE 33—Where low-magnification autographic recordings aremagnification Class C devices is helpful, such as in facilitating needed to facilitate measurement of yield point elongation for materials which may have discontinuous yielding, Class C extensometers may be em- ployed. When this is done but the material exhibits no discontinuous yielding, the extension-under-load yield strength may be determined
E 8M – 04 188.8.131.52 Some materials exhibit a yield point followed by considerable elongation where the yield point is the maximum force achieved during the test. In this case, uniform elongation is not determined at the yield point, but instead at the highest force occurring just prior to necking (see Fig. 26). 184.108.40.206 Stress-strain curves for some materials exhibit a lengthy, plateau-like region in the vicinity of the maximum force. For such materials, determine the uniform elongation at the center of the plateau as indicated in Fig. 27 (see also Note 36 below). NOTE 36—When uniform elongation is being determined digitally, noise in the stress-strain data generally causes many small, local peaks and valleys to be recorded in the plateau region. To accommodate this, the following procedure is recommended: - Determine the maximum force recorded (after discontinuous yielding). - Evaluate the sequence of force values recorded before and after the maximum force. - Digitally define the 9plateau9 as consisting of all consecutive data points wherein the force value is within 0.5% of the magnitude of the peak force value. - Determine the uniform elongation as the strain at the mid-point of the ―plateau.‖ FIG. 23 Stress-Strain Diagram Showing Upper Yield Strength Corresponding with Top of Knee 7.9.4 Discussion—The 0.5% value of Note 36 has been selected arbitrarily. In actual practice, the value should beinstead, using the autographic recording (see Extension-Under-Load selected so as to be the minimum figure that is large enough toMethod). effectively define the force plateau. This may require that the 7.7.4 Halt-of-the-Force Method (for materials exhibiting percentage be about 5 times the amplitude of the forcediscontinuous yielding)—Apply an increasing force to the fluctuations occurring due to noise. Values ranging from 0.1%specimen at a uniform deformation rate. When the force to 1.0 % may be found to work acceptably.hesitates, record the corresponding stress as the upper yield 7.10 Tensile Strength—Calculate the tensile strength bystrength. dividing the maximum force carried by the specimen during NOTE 34—The Halt-of-the-Force Method was formerly known as the tension test by the original cross-sectional area of thethe Halt-of-the-Pointer Method, the Drop-of-the-Beam Method, and specimen.the Halt-of-the-Load Method. NOTE 37—If the upper yield strength is the maximum stress recorded, 7.8 Yield Point Elongation—Calculate the yield point elon- and if the stress-strain curve resembles that of Fig. 26, it is recommendedgation from the stress-strain diagram or data by determining that the maximum stress after discontinuous yielding be reported as thethe difference in strain between the upper yield strength (first tensile strength. Where this may occur, determination of the tensile strength should be in accordance with the agreement between the partieszero slope) and the onset of uniform strain hardening (see involved.definition of YPE and Fig. 24). NOTE 35—The stress-strain curve of a material exhibiting only a hint 7.11 Elongation:of the behavior causing YPE may have an inflection at the onset of 7.11.1 In reporting values of elongation, give both theyielding with no point where the slope reaches zero (Fig. 25). Such a original gage length and the percentage increase. If any devicematerial has no YPE, but may be characterized as exhibiting an other than an extensometer is placed in contact with theinflection. Materials exhibiting inflections, like those with measurable specimen’s reduced section during the test, this shall also beYPE, may, in certain applications, acquire an unacceptable surface noted.appearance during forming. Example: elongation 5 30 % increase ~502mm gage length! (5) 7.9 Uniform Elongation (if required): 7.9.1 Uniform elongation shall include both plastic and NOTE 38—Elongation results are very sensitive to variables such as:elastic elongation. ( a) speed of testing, (b) specimen geometry (gage length, diameter, width, and thickness), (c) heat dissipation (through grips, extensometers, or other 7.9.2 Uniform elongation shall be determined using auto- devices in contact with the reduced section), (d) surface finish in reducedgraphic methods with extensometers conforming to Practice section (especially burrs or notches), (e) alignment, and (f) filletsE 83. Use a class B2 or better extensometer for materials and tapers. Parties involved in comparison or conformance testinghaving a uniform elongation less than 5 %. Use a class C or should standardize the above items, and it is recommended that use ofbetter extensometer for materials having a uniform elongation ancillary devices (such as extensometer supports) which may removegreater than or equal to 5 % but less than 50 %. Use a class D heat from specimens be avoided. See Appendix X1. for additional information on the effects of these variables.or better extensometer for materials having a uniform elonga-tion of 50 % or greater. 7.11.2 When the specified elongation is greater than 3 %, fit 7.9.3 Determine the uniform elongation as the elongation at ends of the fractured specimen together carefully and measurethe point of maximum force from the force elongation data the distance between the gage marks to the nearest 0.25 mm forcollected during a test. 15
E 8M – 04 FIG. 24 Stress-Strain Diagram Showing Yield Point Elongation and Upper and Lower Yield Strengthsgage lengths of 50 mm and under, and to at least the nearest and non-representative of the material. If such an elongation0.5 % of the gage length for gage lengths over 50 mm. A measure is obtained in acceptance testing involving only apercentage scale reading to 0.5 % of the gage length may be minimum requirement and meets the requirement, no furtherused. testing need be done. Otherwise, discard the test and retest the 7.11.3 When the specified elongation is 3 % or less, deter- material.mine the elongation of the specimen using the following 7.11.5 Elongation at fracture is defined as the elongationprocedure, except that the procedure given in 7.11.2 may be measured just prior to the sudden decrease in force associatedused instead when the measured elongation is greater than 3 %. with fracture. For many ductile materials not exhibiting a 220.127.116.11 Prior to testing, measure the original gage length of sudden decrease in force, the elongation at fracture can bethe specimen to the nearest 0.05 mm. taken as the strain measured just prior to when the force falls 18.104.22.168 Remove partly torn fragments that will interfere below 10 % of the maximum force encountered during the test.with fitting together the ends of the fractured specimen or with 22.214.171.124 Elongation at fracture shall include elastic andmaking the final measurement. plastic elongation and may be determined with autographic or 126.96.36.199 Fit the fractured ends together with matched sur- automated methods using extensometers verified over thefaces and apply a force along the axis of the specimen sufficient strain range of interest (see 5.4). Use a class B2 or betterto close the fractured ends together. If desired, this force may extensometer for materials having less than 5 % elongation, athen be removed carefully, provided the specimen remains class C or better extensometer for materials having elongationintact. greater than or equal to 5 % but less than 50 %, and a class D NOTE 39—The use of a force of approximately 15 MPa has been or better extensometer for materials having 50 % or greaterfound to give satisfactory results on test specimens of aluminum alloy. elongation. In all cases, the extensometer gage length shall be 188.8.131.52 Measure the final gage length to the nearest 0.05 the nominal gage length required for the specimen being tested.mm and report the elongation to the nearest 0.2 %. Due to the lack of precision in fitting fractured ends together, 7.11.4 Elongation measured per paragraph 7.11.2 or 7.11.3 the elongation after fracture using the manual methods of themay be affected by location of the fracture, relative to the preceding paragraphs may differ from the elongation at fracturemarked gage length. If any part of the fracture occurs outside determined with extensometers.the gage marks or is located less than 25 % of the elongated 184.108.40.206 Percent elongation at fracture may be calculatedgage length from either gage mark, the elongation value directly from elongation at fracture data and be reportedobtained using that pair of gage marks may be abnormally low instead of percent elongation as calculated in paragraphs 7.11.2 16
E 8M – 04 FIG. 25 Stress-Strain Diagram With an Inflection, But No YPEto 7.11.3. However, these two parameters are not interchange- and t3 are the thicknesses at the corners, and t2 is the thickness atable. Use of the elongation at fracture method generally the mid-width. An effective width may be similarly calculated.provides more repeatable results. 7.12.4 Calculate the reduced area based upon the dimen- NOTE 40—When disagreements arise over the percent elongation re- sions determined in 7.12.2 or 7.12.3. The difference betweensults, agreement must be reached on which method to use to obtain the the area thus found and the area of the original cross sectionresults. expressed as a percentage of the original area is the reduction 7.12 Reduction of Area: of area. 7.12.1 The reduced area used to calculate reduction of area 7.12.5 If any part of the fracture takes place outside the(see 7.12.2 and 7.12.3) shall be the minimum cross section at middle half of the reduced section or in a punched or scribedthe location of fracture. gage mark within the reduced section, the reduction of area 7.12.2 Specimens With Originally Circular Cross value obtained may not be representative of the material. InSections—Fit the ends of the fractured specimen together and acceptance testing, if the reduction of area so calculated meetsmeasure the reduced diameter to the same accuracy as the the minimum requirements specified, no further testing isoriginal measurement. required, but if the reduction of area is less than the minimum NOTE 41—Because of anisotropy, circular cross sections often do requirements, discard the test results and retest.not remain circular during straining in tension. The shape is usually 7.12.6 Results of measurements of reduction of area shall beelliptical, thus, the area may be calculated by p· d1·d2/4, where d 1 andd2 are the major and minor diameters, respectively. rounded using the procedures of Practice E 29 and any specific procedures in the product specifications. In the absence of a 7.12.3 Specimens With Originally Rectangular Cross specified procedure, it is recommended that reduction of areaSections—Fit the ends of the fractured specimen together and test values in the range from 0 to 10 % be rounded to themeasure the thickness and width at the minimum cross section nearest 0.5 % and test values of 10 % and greater to the nearestto the same accuracy as the original measurements. 1 %. NOTE 42—Because of the constraint to deformation that occurs at 7.13 Rounding Reported Test Data for Yield Strength andthe corners of rectangular specimens, the dimensions at the center of Tensile Strength—Test data should be rounded using thethe original flat surfaces are less than those at the corners. The shapes ofthese surfaces are often assumed to be parabolic. When this assumption is procedures of Practice E 29 and the specific procedures in themade, an effective thickness, te, may be calculated by: (t1 + 4t 2 + t3)/6, product specifications. In the absence of a specified procedurewhere t1 17
E 8M – 04 FIG. 26 Stress-Strain Diagram in Which the Upper Yield Strength is the Maximum Stress Recorded 7.13.2 For all test values, round to the nearest 1 MPa. NOTE 44—For aluminum- and magnesium-alloy products, see Methods B 557M. 7.13.3 For all test values, round to the nearest 5 MPa. 7.14 Replacement of Specimens—A test specimen may be discarded and a replacement specimen selected from the same lot of material in the following cases: 7.14.1 The original specimen had a poorly machined sur- face, 7.14.2 The original specimen had the wrong dimensions, 7.14.3 The specimen’s properties were changed because of poor machining practice, 7.14.4 The test procedure was incorrect, 7.14.5 The fracture was outside the gage length, 7.14.6 For elongation determinations, the fracture was out- FIG. 27 Load-Strain Diagram for Determination of Uniform side the middle half of the gage length, or Elongation of Steel Sheet Materials Exhibiting a Plateau at 7.14.7 There was a malfunction of the testing equipment. Maximum Load NOTE 45—The tension specimen is inappropriate for assessing some types of imperfections in a material. Other methods and specimens employing ultrasonics, dye penetrants, radiography, etc., mayfor rounding the test data, one of the procedures described in be consid- ered when flaws such as cracks, flakes, porosity, etc., arethe following paragraphs is recommended. revealed during a test and soundness is a condition of acceptance. 7.13.1 For test values up to 500 MPa, round to the nearest 1MPa; for test values of 500 MPa and up to 1000 MPa, round to 8. Reportthe nearest 5 MPa; for test values of 1000 MPa and greater, 8.1 Test information on materials not covered by a productround to the nearest 10 MPa. specification should be reported in accordance with 8.2 or both NOTE 43—For steel products, see Test Methods and Definitions A 370. 8.2 and 8.3. 18
E 8M – 04 8.2 Test information to be reported shall include the follow- Tensile Yield Yield Elongation Reductioning when applicable: Strength Strength Strength Gage Length of Area Off- Offset = 0.2 % = 5 Diam- 8.2.1 Material and sample identification. set = 0.02 % eters 8.2.2 Specimen type (Section 6). CV% r 0.9 2.7 1.4 3.0 2.8 8.2.3 Yield strength and the method used to determine yield CV% R 1.3 4.5 2.3 6.4 4.6 CV% r = repeatability coefficient of variation in percent within a laboratorystrength (see 7.7). CV %R = repeatability coefficient of variation in percent between laboratories 8.2.4 Yield point elongation (see 7.8). 8.2.5 Tensile strength (see 7.10). 9.1.1 The values shown are the averages from tests on six 8.2.6 Elongation (report original gage length, percentage frequently tested metals, selected to include most of the normalincrease, and method used to determine elongation) (see 7.11). range for each property listed above. When these materials are 8.2.7 Reduction of area, if required (see 7.12). compared, a large difference in coefficient of variation is found. 8.3 Test information to be available on request shall include: Therefore, the values above should not be tightness; width; 8.3.1 Specimen test section dimension(s). workmanship used to judge whether the difference between 8.3.2 Formula used to calculate cross-sectional area of duplicate tests of a specific material is larger than expected.specimens taken from large-diameter tubular products. The values are provided to allow potential users of this test 8.3.3 Speed and method used to determine speed of testing method to assess, in general terms, its usefulness for a(see 7.6). proposed application. 8.3.4 Method used for rounding of test results (see 7.13). 9.2 Bias—The procedures in Test Methods E 8M for mea- 8.3.5 Reasons for replacement specimens (see 7.14). suring tensile properties have no bias because these properties can only be defined in terms of a test method.9. Precision and Bias 3 10. Keywords 9.1 Precision—An interlaboratory test program gave the 10.1 accuracy; bending stress; discontinuous yielding; drop-following values for coefficients of variation for the most of-the-beam; eccentric force application; elastic extension;commonly measured tensile properties: elongation; extension-under-load; extensometer; force; free-Coefficient of Variation, % running crosshead speed; gage length; halt-of-the force; per- cent elongation; plastic extension; preload; rate of stressing; rate of straining; reduced section; reduction of area; sensitivity; 3 Supporting data can be found in Appendix I and additional data are available strain; stress; taring; tensile strength; tension testing; yieldfrom ASTM Headquarters. Request RR: E28-1004 and E28-1006. point elongation; yield strength APPENDIXES (Nonmandatory Information) X1. FACTORS AFFECTING TENSION TEST RESULTS X1.1 The precision and bias of tension test strength and representativeness and homogeneity of the test material, sam-ductility measurements depend on strict adherence to the stated pling scheme, and specimen preparation (surface finish, dimen-test procedure and are influenced by instrumental and material sional accuracy, fillets at the ends of the gage length, taper infactors, specimen preparation, and measurement/testing errors. the gage length, bent specimens, thread quality, and so forth). X1.2 The consistency of agreement for repeated tests of the X1.4.1 Some materials are very sensitive to the quality ofsame material is dependent on the homogeneity of the material, the surface finish of the test specimen (see Note 8) and must beand the repeatability of specimen preparation, test conditions, ground to a fine finish, or polished to obtain correct results.and measurements of the tension test parameters. X1.4.2 Test results for specimens with as-cast, as-rolled, as-forged, or other non-machined surface conditions can be X1.3 Instrumental factors that can affect test results in- affected by the nature of the surface (see Note 14).clude: the stiffness, damping capacity, natural frequency, and X1.4.3 Test specimens taken from appendages to the part ormass of moving parts of the tensile test machine; accuracy of component, such as prolongs or risers, or from separatelyforce indication and use of forces within the verified range of produced castings (for example, keel blocks) may produce testthe machine; rate of force application, alignment of the test results that are not representative of the part or component.specimen with the applied force, parallelness of the grips, grippressure, nature of the force control used, appropriateness and X1.4.4 Test specimen dimensions can influence test results.calibration of extensometers, heat dissipation (by grips, exten- For cylindrical or rectangular specimens, changing the testsometers, or ancillary devices), and so forth. specimen size generally has a negligible effect on the yield and tensile strength but may influence the upper yield strength, if X1.4 Material factors that can affect test results include: one is present, and elongation and reduction of area values. 19
E 8M – 04Comparison of elongation values determined using different X1.5.2 Materials with anisotropic flow characteristics mayspecimens requires that the following ratio be controlled: exhibit non-circular cross sections after fracture and measure- ment precision may be affected, as a result (see Note 37). L0/ ~A 0 !1 / 2 (X1.1) X1.5.3 The corners of rectangular test specimens are subject where: to constraint during deformation and the originally flat surfaces L0 = original gage length of specimen, and may be parabolic in shape after testing which will affect the A0 = original cross-sectional area of specimen. precision of final cross-sectional area measurements (see Note X220.127.116.11 Specimens with smaller L0/ ( A0) ⁄ ratios generally 1 2 42).give greater elongation and reduction in area values. This is the X1.5.4 If any portion of the fracture occurs outside of thecase, for example, when the width or thickness of a rectangular middle of the gage length, or in a punch or scribe mark withintensile test specimen is increased. the gage length, the elongation and reduction of area values X18.104.22.168 Holding the L0/( A0) ⁄ ratio constant minimizes, 1 2 may not be representative of the material. Wire specimens thatbut does not necessarily eliminate, differences. Depending on break at or within the grips may not produce test resultsmaterial and test conditions, increasing the size of the propor- representative of the material.tional specimen of Fig. 8 may be found to increase or decrease X1.5.5 Use of specimens with shouldered ends (―button-elongation and reduction in area values somewhat. head‖ tensiles) will produce lower 0.02 % offset yield strength X1.4.5 Use of a taper in the gage length, up to the allowed values than threaded specimens.1 % limit, can result in lower elongation values. Reductions ofas much as 15 % have been reported for a 1 % taper. X1.6 Because standard reference materials with certified X1.4.6 Changes in the strain rate can affect the yield tensile property values are not available, it is not possible tostrength, tensile strength, and elongation values, especially for rigorously define the bias of tension tests. However, by the usematerials which are highly strain rate sensitive. In general, the of carefully designed and controlled interlaboratory studies, ayield strength and tensile strength will increase with increasing reasonable definition of the precision of tension test results canstrain rate, although the effect on tensile strength is generally be obtained.less pronounced. Elongation values generally decrease as the X1.6.1 An interlaboratory test program, (see footnote 7),strain rate increases. was conducted in which six specimens each, of six different X1.4.7 Brittle materials require careful specimen prepara- materials were prepared and tested by each of six differenttion, high quality surface finishes, large fillets at the ends of the laboratories. Tables X1.1-X1.5 present the precision statistics,gage length, oversize threaded grip sections, and cannot as defined in Practice E 691, for: tensile strength, 0.02 % yieldtolerate punch or scribe marks as gage length indicators. strength, 0.2 % yield strength, % elongation in 5D, and % X1.4.8 Flattening of tubular products to permit testing does reduction in area. In each table, the first column lists the sixalter the material properties, generally nonuniformity, in the materials tested, the second column lists the average of theflattened region which may affect test results. average results obtained by the laboratories, the third and fifth columns list the repeatability and reproducibility standard X1.5 Measurement errors that can affect test results in- deviations, the fourth and sixth columns list the coefficients ofclude: verification of the test force, extensometers, microme- variation for these standard deviations, and the seventh andters, dividers, and other measurement devices, alignment and eighth columns list the 95 % repeatability and reproducibilityzeroing of chart recording devices, and so forth. limits. X1.5.1 Measurement of the dimensions of as-cast, as-rolled, X1.6.2 The averages (below columns four and six in eachas-forged, and other test specimens with non-machined sur- table) of the coefficients of variation permit a relative compari-faces may be imprecise due to the irregularity of the surface son of the repeatability (within-laboratory precision) andflatness. reproducibility (between-laboratory precision) of the tension TABLE X1.1 Precision Statistics—Tensile Strength, MPa NOTE 1— X is the average of the cell averages, that is, the grand mean for the testparameter, sr is the repeatability standard deviation (within-laboratory precision),sr/X is the coefficient of variation in %,sR is the reproducibility standard deviation (between-laboratory precision),sR/X is the coefficient of variation, %,r is the 95 % repeatability limits,R is the 95 % reproducibility limits. Material X sr s r /X,% sR sR/X, % r R EC-H19 176.9 4.3 2.45 4.3 2.45 12.1 12.1 2024-T351 491.3 6.1 1.24 6.6 1.34 17.0 18.5 ASTM A105 596.9 4.1 0.69 8.7 1.47 11.6 24.5 AISI 316 694.6 2.7 0.39 8.4 1.21 7.5 23.4 Inconel 600 685.9 2.9 0.43 5.0 0.72 8.2 13.9 SAE 51410 1253.0 3.2 0.25 7.9 0.63 8.9 22.1 Averages: 0.91 1.30 20
E 8M – 04 TABLE X1.2 Precision Statistics—0.02 % Yield Strength, MPa Material X sr s r /X,% sR sR/X, % r R EC-H19 111.4 4.5 4.00 8.2 7.37 12.5 23.0 2024-T351 354.2 5.8 1.64 6.1 1.73 16.3 17.2 ASTM A105 411.4 8.3 2.02 13.1 3.18 23.2 36.6 AISI 316 336.1 16.7 4.97 31.9 9.49 46.1 89.0 Inconel 600 267.1 3.2 1.18 5.2 1.96 8.8 14.7 SAE 51410 723.2 16.6 2.29 21.9 3.02 46.4 61.2 Averages: 2.68 4.46 TABLE X1.3 Precision Statistics—0.2 % Yield Strength, MPa Material X sr s r /X,% sR sR/X, % r R EC-H19 158.4 3.3 2.06 3.3 2.07 9.2 9.2 2024-T351 362.9 5.1 1.41 5.4 1.49 14.3 15.2 ASTM A105 402.4 5.7 1.42 9.9 2.47 15.9 27.8 AISI 316 481.1 6.6 1.36 19.5 4.06 18.1 54.7 Inconel 600 268.3 2.5 0.93 5.8 2.17 7.0 16.3 SAE 51410 967.5 8.9 0.92 15.9 1.64 24.8 44.5 Averages: 1.35 2.32 TABLE X1.4 Precision Statistics— % Elongation in 5D NOTE 1—Length of reduced section = 6D. Material X sr sr/X,% sR sR/X, % r R EC-H19 14.60 0.59 4.07 0.66 4.54 1.65 1.85 2024-T351 17.99 0.63 3.48 1.71 9.51 1.81 4.81 ASTM A105 25.63 0.77 2.99 1.30 5.06 2.15 3.63 AISI 316 35.93 0.71 1.98 2.68 7.45 2.00 7.49 Inconel 600 41.58 0.67 1.61 1.60 3.86 1.88 4.49 SAE 51410 12.39 0.45 3.61 0.96 7.75 1.25 2.69 Averages: 2.96 6.36 TABLE X1.5 Precision Statistics— % Reduction in Area Material X sr s r /X,% sR sR/X, % r R EC-H19 79.15 1.93 2.43 2.01 2.54 5.44 5.67 2024-T351 30.41 2.09 6.87 3.59 11.79 5.79 10.01 ASTM A105 65.59 0.84 1.28 1.26 1.92 2.35 3.53 AISI 316 71.49 0.99 1.39 1.60 2.25 2.78 4.50 Inconel 600 59.34 0.67 1.14 0.70 1.18 1.89 1.97 SAE 51410 50.49 1.86 3.69 3.95 7.81 5.21 11.05 Averages: 2.80 4.58test parameters. This shows that the ductility measurements X1.6.3 No comments about bias can be made for theexhibit less repeatability and reproducibility than the strength interlaboratory study due to the lack of certified test results formeasurements. The overall ranking from the least to the most these specimens. However, examination of the test resultsrepeatable and reproducible is: % elongation in 5D, % reduc- showed that one laboratory consistently exhibited higher thantion in area, 0.02 % offset yield strength, 0.2 % offset yield average strength values and lower than average ductility valuesstrength, and tensile strength. Note that the rankings are in the for most of the specimens. One other laboratory had consis-same order for the repeatability and reproducibility average tently lower than average tensile strength results for allcoefficients of variation and that the reproducibility (between- specimens.laboratory precision) is poorer than the repeatability (within-laboratory precision), as would be expected. 21
E 8M – 04 X2. MEASUREMENT OF SPECIMEN DIMENSIONS X2.1 Measurement of specimen dimensions is critical in X2.7 Factors which affect GR and R, sometimes dramati-tension testing, and it becomes more critical with decreasing cally, and which should be considered in the selection andspecimen size, as a given absolute error becomes a larger evaluation of hardware and procedures include:relative (percent) error. Measuring devices and procedures X2.7.1 Resolution,should be selected carefully, so as to minimize measurement X2.7.2 Verification,error and provide good repeatability and reproducibility. X2.7.3 Zeroing, X2.2 Relative measurement error should be kept at or X2.7.4 Type of anvil (flat, rounded, or pointed),below 1 %, where possible. Ideally, this 1 % error should X2.7.5 Cleanliness of part and anvil surfaces, X2.7.6 User-friendliness of measuring device,include not only the resolution of the measuring device but also X2.7.7 Stability/temperature variations,the variability commonly referred to as repeatability andreproducibility. (Repeatability is the ability of any operator to X2.7.8 Coating removal,obtain similar measurements in repeated trials. Reproducibility X2.7.9 Operator techique, and X2.7.10 Ratchets or other features used to regulate theis the ability of multiple operators to obtain similar measure- clamping force.ments.) X2.3 Formal evaluation of gage repeatability and reproduc- X2.8 Flat anvils are generally preferred for measuring theibility (GR and R) by way of a GR and R study is highly dimensions of round or flat specimens which have relativelyrecommended. A GR and R study involves having multiple smooth surfaces. One exception is that rounded or pointedoperators each take two or three measurements of a number of anvils must be used in measuring the thickness of curvedparts—in this case, test specimens. Analysis, usually done by specimens taken from large-diameter tubing (see Fig. 13), tocomputer, involves comparing the observed measurement prevent overstating the thickness. (Another concern for thesevariations to a tolerance the procedure is to determine con- curved specimens is the error that can be introduced throughformance to. High GR and R percentages (more than 20 %) use of the equation A = W 3 T; see 7.2.3.)indicate much variability relative to the tolerance, whereas low X2.9 Heavy coatings should generally be removed from atpercentages (10 % or lower) indicate the opposite. The analysis least one grip end of flat specimens taken from coated productsalso estimates, independently, the repeatability and reproduc- to permit accurate measurement of base metal thickness,ibility. assuming (a) the base metal properties are what are desired, (b) X2.4 GR and R studies in which nontechnical personnel the coating does not contribute significantly to the strength ofused different brands and models of hand-held micrometers the product, and (c) coating removal can be easily accom-have given results varying from about 10 % (excellent) to plished (some coatings may be easily removed by chemicalnearly 100 % (essentially useless), relative to a dimensional stripping). Otherwise, it may be advisable to leave the coatingtolerance of 0.075 mm. The user is, therefore, advised to be intact and determine the base metal thickness by an alternatevery careful in selecting devices, setting up measurement method. Where this issue may arise, all parties involved inprocedures, and training personnel. comparison or conformance testing should agree as to whether or not coatings are to be removed before measurement. X2.5 With a 0.075 mm tolerance, a 10 % GR and R result(exceptionally good, even for digital hand-held micrometers X2.10 As an example of how the considerations identifiedreading to 0.001 mm) indicates that the total variation due to above affect dimensional measurement procedures, considerrepeatability and reproducibility is around 0.0075 mm. This is the case of measuring the thickness of 0.40 mm painted, flatless than or equal to 1 %, only if all dimensions to be measured rolled steel specimens. The paint should be removed prior toare greater than or equal to 0.75 mm. The relative error in using measurement, if possible. The measurement device usedthis device to measure thickness of a 0.25 mm flat tensile should have flat anvils, must read to 0.001 mm or better, andspecimen would be 3 %, which is considerably more than that must have excellent repeatability and reproducibility. Since GRallowed for load or strain measurement. and R is a significant concern, it will be best to use a device which has a feature for regulating the clamping force used, and X2.6 Dimensional measurement errors can be identified as devices without digital displays should be avoided to preventthe cause of many out-of-control signals, as indicated by reading errors. Before use of the device, and periodicallystatistical process control (SPC) charts used to monitor tension during use, the anvils should be cleaned, and the device shouldtesting procedures. This has been the experience of a produc- be verified or zeroed (if an electronic display is used) or both.tion laboratory employing SPC methodology and the best Finally, personnel should be trained and audited periodically tohand-held micrometers available (from a GR and R standpoint) ensure that the measuring device is being used correctly andin testing of 0.45 mm to 6.35 mm flat-rolled steel products. consistently by all. 22
E 8M – 04 X3. SUGGESTED ACCREDITATION CRITERIA FOR LABORATORIES PERFORMING TENSILE TESTSX3.1 Scope X3.4 Procedures X3.1.1 The following are specific features that an assessor X3.4.1 The test machine shall be set up and zeroed in suchmay check to assess a laboratory’s technical competence, if the a manner that zero force indication signifies a state of zerolaboratory is performing tests in accordance with Test Methods force on the specimen, as indicated in the Zeroing of the TestE 8 and/or E 8M. Machine sections of Test Methods E 8 and E 8M. NOTE X3.2—Provisions should be made to ensure that zero readingsX3.2 Preparation are properly maintained, from test to test. These may include, for X3.2.1 The laboratory should follow documented proce- example, zeroing after a predetermined number of tests or each time, under zero force conditions, the indicator exceeds a predetermineddures to ensure that machining or other preparation generates value.specimens conforming to applicable tolerances and require-ments of Test Methods E 8 or E 8M. Particularly important are X3.4.2 Upon request, the laboratory should be capable ofthose requirements that pertain to the dimensions and finish of demonstrating (perhaps through time, force, displacement orreduced sections, as found in the text and in applicable figures. extensometer measurements, or both) that the test speeds used X3.2.2 Where gage marks are used, the laboratory should conform to the requirements of Test Methods E 8 or E 8M, oremploy documented gage marking procedures to ensure that other standards which take precedence.the marks and gage lengths comply with the tolerances and X3.4.3 Upon request, the laboratory should be capable ofguidelines of Test Methods E 8 or E 8M. demonstrating that the offsets and extensions used in determin- ing yield strengths conform to the requirements of Test X22.214.171.124 The gage marking procedure used should notdeleteriously affect the test results. Methods E 8 or E 8M and are constructed so as to indicate the forces corresponding to the desired offset strain or total strain. NOTE X3.1—Frequent occurrence of fracturing at the gage marksmay indicate that gage marks have excessive depth or sharpness and NOTE X3.3—Use caution when performing calculations withmay be affecting test results. exten- someter magnification, because the manufacturer may report strain mag- nification, which relates the strain (not the elongation) to the x-axis displacement on the stress strain diagram. A user or assessorX3.3 Test Equipment interested in an extensometer’s magnification may use calibration X3.3.1 As specified in the Apparatus sections of Test equipment to deter- mine the ratio between elongation and chartMethods E 8 and E 8M, the axis of the test specimen should travel or may verify a reported magnification by calculating thecoincide with the center line of the heads of the testing Young’s modulus from tests of specimens of a known nominal modulus.machine, in order to minimize bending stresses which could X3.4.4 Measurement of elongation shall conform to re-affect the results. quirements of Test Methods E 8 or E 8M. X3.3.2 Equipment verification requirements of Practices NOTE X3.4—Test Methods E 8 and E 8M permit the measurementE 4 and E 83 shall be met. Documentation showing the and reporting of elongation at fracture in place of elongation, as is oftenverification work to have been thorough and technically correct done in automated testing.should be available. X3.4.5 Reduction of area, when required, shall be deter- X126.96.36.199 Verification reports shall demonstrate that force mined in accordance with the requirements of Test Methodsand extension readings have been taken at the prescribed E 8 or E 8M.intervals and that the prescribed runs have been completed. X3.4.6 Procedures for recording, calculating, and reporting X3.3.3 Extensometers used shall meet all requirements of data and test results shall conform to all applicable require-Test Methods E 8 or E 8M as to the classification of device to ments of Test Methods E 8 or E 8M. In addition, whereverbe used for the results determined. For example, an extensom- practical, the procedures should also be in accordance witheter not meeting the Class B2 requirements of Practice E 83 widely accepted provisions of good laboratory practice, such asmay not be used in determination of offset yield strengths. those detailed below. X3.3.4 Before computerized or automated test equipment is X188.8.131.52 When recording data, personnel should record allput into routine service, or following a software revision, it is figures that are definite, plus the best estimate of the first figurerecommended that measures be taken to verify proper opera- which is uncertain. (If a result is known to be approximatelytion and result interpretation. Guide E 1856 addresses this midway between 26 and 27, 26.5 should be the result recordedconcern. (not 26, 27, or 26.475). X3.3.5 Micrometers and other devices used in measurement X184.108.40.206 When performing calculations, personnel shouldof specimen dimensions should be selected, maintained and avoid compounding of rounding errors. This may be accom-used in such a manner as to comply with the appendixes of Test plished by performing one large calculation, rather than severalMethods E 8 and E 8M on measurement. Traceability to calculations using individual results. Alternatively, if multi-national standards should be established for these devices, and step calculations are done, intermediate results should not bereasonable effort should be employed to prevent errors greater rounded before use in subsequent calculations.than 1 % from being generated as a result of measurement X220.127.116.11 In rounding, no final result should retain moreerror, resolution, and rounding practice. significant figures than the least-significant-figure measure- ment or data point used in the calculation. 23
E 8M – 04X3.5 Retention tensile testing. These instructions should be readily available to X3.5.1 A retention program appropriate for the nature and all qualified operators.frequency of testing done in the laboratory should be main- X3.7.3 All applicable verification requirements shall betained. Items that may warrant retention for defined time met, as detailed in X3.3.2.periods include: X3.7.4 It is recommended that special studies and programs X18.104.22.168 Raw data and forms, be employed to monitor and control tensile testing, because X22.214.171.124 Force-elongation or stress-strain charts, X126.96.36.199 tensile test results are easily affected by operators, measuring Computer printouts of curves and test results, X188.8.131.52 devices, and test equipment. Examples of such programs Data and results stored on computer discs or hard include but are not limited to:drives, X184.108.40.206 Round-robin studies, proficiency tests, or other X220.127.116.11 Broken specimens, cross-checks, X18.104.22.168 Excess material, X22.214.171.124 Test reports, and X126.96.36.199 Repeatability and reproducibility (R and R) stud- X188.8.131.52 Verification reports and certifications. ies, X184.108.40.206 Control charting, andX3.6 Environment X220.127.116.11 Determination of typical lab uncertainties for each X3.6.1 All test equipment should be located and connected result typically reported.to power sources in such a manner as to minimize the effectsof vibrations and electrical disturbances on raw data collected, NOTE X3.5—For nondestructive testing, repeatability andstress-strain charts, and operation of equipment. reproducibil- ity are often measured by conducting gage R and R studies, as discussed in Appendix X2 of Test Methods E 8 and E 8M. TheseX3.7 Controls studies involve repeated determination of a test result, using a single part or specimen, so gage R and Rs are not directly applicable to mechanical X3.7.1 Controlled procedures and work instructions should properties, which are obtained through destructive testing. (Truecover all aspects of specimen preparation, tensile testing, and differences between even the best duplicate specimens manifestresult reporting. These documents should be readily available themselves in the form of poorer R and R results than would be obtainedto all involved in the documented tasks. for perfect duplicates.) Nevertheless, quasi-R and R studies conducted X3.7.2 Clear, concise, operating instructions should be with these limitations taken into consideration may be helpful inmaintained for equipment used in specimen preparation and analyzing sources of error and improving reliability of test results. SUMMARY OF CHANGES Committee E28 has identified the location of selected changes to this standard since the last issue (E 8M – 03) that may impact the use of this standard. (Approved July 10, 2003)(1) Section 18.104.22.168 was revised. Note 36 and a discussion wereadded following this revised section. Committee E28 has identified the location of selected changes to this standard since the last issue (E 8M – 01) that may impact the use of this standard. (Approved Oct. 10, 2001)(1) Section 6.5 and it subsections were revised. (3) Appendix X3 was added.(2) Note 10 was deleted and the remaining notes wererenumbered. ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every five years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or firstname.lastname@example.org (e-mail); or through the ASTM website (www.astm.org). 24
5. DIBUJOS5.1 DIBUJO DE LA MAQUINA
5.2 DIBUJO DE LA PROBETA ANTES DELENSAYO.
5.3 DIBUJO DE LA PROBETA DESPUES DEL ENSAYO.
6. TABLA DE DATOS La tabla de datos se genera mientras la carga aumenta de 500 en 500, hasta llegar a lacarga máxima y punto de fractura. A relación es carga proporcional a cm de desplazamiento
7. CALCULOSES EL PRIMER ESFUERZO EN EL CUAL EL MATERIAL DESARROLLA UN MARCADO INCREMENTO DE LA DEFORMACIONSIN AUMENTAR EL ESFUERZO.a) Esfuerzo de cedencia.MAYOR ESFUERZO BASADO EN LA SECCION ORIGINAL.b) Esfuerzo máximo.CONSTANTE DE PROPORCIONALIDAD DE LOS ESFUERZOS A LAS DEFORMACIONES ES LA PENDIENTE DE LA LÍNEAc) Modulo de elasticidad.SE OBTIENE COMPARANDO EL ALARGAMIENTO TOTAL EN LA FRACTURA CON LA LONGITUD CALIBRADAd) Porcentaje de alargamiento.SE OBTIENE COMPARANDO LA REDUCCION DEL ÁREA EN LA SECCION MAS PEQUEÑA DE LA PROBETA FRACTURADACON EL ÁREA DE LA SECCION TRANSVERSAL ORIGINALe) Porcentaje de reducción de área.ES LA CANTIDAD DE ENERGÍA POR UNIDAD DE VOLUMEN FUE UN MATERIAL PUEDE ABSORBERELÁSTICAMENTE.f) Modulo de resistencia.
ES LA CANTIDAD DE ENERGÍA POR UNIDAD DE VOLUMEN QUE PUEDE ABSORBER UN MATERIAL ANTES DE LAFRACTURA.g) Modulo de tenacidad.7. GRAFICADIAGRAMA ESFUERZO-DEFORMACIÓN ESFUERZO UNITARIO 4 3,5 3 2,5 2 δ 1,5 1 0,5 0 -0,5 0 2000 4000 6000 8000 10000 12000 LOAD kg
1. LOS VALORES DEL ESFUERZO UNITARIO (cr) SE CALCULA DIVIDIENDO LOS VALORES DE LA CARGA (P) ENTRE EL ÁREADE LA SECCIÓN ORIGINAL DE LA PROBETA (Ao)2, LOS VALORES DE LA DEFORMACIÓN UNITARIA (E) SE CALCULA DIVIDIÉNDOLO LOS VALORES DEL ALARGAMIENTO (8)ENTRE LA LONGITUD CALIBRADA8. TABLA DE RESULTADOS
9. CUESTIONARIO1.- De acuerdo a las fracturas por tensión ordene y mencione como se clasifican: b) c) d) e) a) f)2.-Mencione y grafique las características del diagrama esfuerzo– desplazamiento3.-Coloque los tipos de mordazas para ensayos de tensión.4.-Mencione y enumere las propiedades mecánicas para el ensayo de tensión.5.- Explique brevemente el siguiente diagrama:6. Mencione las habilidades obtenidas durante el desarrollo de la práctica.7.-Explique las características del control del ensayo de tensión8.-Mencione realizando un mapa conceptual las aplicaciones a nivel industrial el ensayo de tensión.9.-Mencione y coloque los tipos de extensómetros para las lecturas del desplazamiento.10. Conceptualice las ventajas y desventajas en el uso y aplicación del ensayo según la normaASTM E-8.
11. BIBLIOGRAFIAEnsaye e Inspección de los Materiales enIngenieríaHARMER E. DAVID
GEORGE EARL TROXELLCLEMENT T WISKOCILEDIT.C.E.C.S.A MÉXICOPAG: 155-184